effect of temperature, heating rate and zeolite-based ...poj.ippi.ac.ir/article_1577_6a6fb0d89c83...
Post on 29-Mar-2020
Embed Size (px)
Polyolefins Journal, Vol. 6, No. 1 (2019) IPPI DOI: 10.22063/poj.2018.2189.1114
Effect of temperature, heating rate and zeolite-based catalysts on the pyrolysis of high impact polystyrene
(HIPS) waste to produce fuel-like products
Zaher Tamri1, Ali Vaziri Yazdi1*, Mehdi Nekoomanesh Haghighi2, Mehrdad Seifali Abbas-Abadi2, Amir Heidarinasab1
1Department of Chemical Engineering, Science and Research Branch, Islamic Azad University, Tehran, Iran 2Department of Polymerization Engineering, Iran Polymer and Petrochemical Institute, Tehran, Iran
Received: 4 May 2018, Accepted: 18 August 2018
Pyrolysis of high impact polystyrene (HIPS) waste has been investigated under different process parameters, such as temperature, heating rate and types of zeolitic catalysts to produce valuable liquid products. Liquid, gas and coke as products of pyrolysis and aromatic, naphthene, olefin and paraffin as liquid components were obtained and their molecular weight distributions were studied with changing the process parameters in a stirred reactor. Aromatic-rich hydrocarbons within the gasoline range were the main pyrolysis products. Type of zeolitic catalysts, temperature and heating rate had significant effects on the products quality and quantity. Non-isothermal mass losses of high impact polystyrene were measured using a thermo-gravimetric analyzer (TGA) at heating rates of 5, 15, 30, 45 and 90°C min-1 until the furnace wall temperature reached 600°C. The DTG (differential thermal gravimetric) curves showed that heating rate had no obvious effect on the degradation trends in the studied range, and by increasing heating rate, the activation energies were decreased obviously from 222.5 to183.6 kJ mol-1. Polyolefins J (2019) 6: 43-52
Keywords: High impact polystyrene; temperature; heating rate; catalyst; TGA.
* Corresponding Author - E-mail: email@example.com
High impact polystyrene (HIPS) is the copolymer of polystyrene and butadiene rubber with improved toughness in comparison with polystyrene. Butadiene rubber as dispersed rubber phase in the polystyrene media with great increase in impact strength and environmental stress cracking resistance (ESCR) has led to a considerable growth in the range of applications for this polymer [1-2], including refrigeration cabinets, general packaging, electronics, toys, household appliances and disposables.
The increasing growth of HIPS waste can cause a lot of environmental problems in the related industries. On the other hand, HIPS waste has high volatile, fixed carbon and aromatic enriched content with heating value greater than the classic fuels. The understanding of effect of effective parameters on the thermal degradation processes, especially pyrolysis and gasification of various HIPS wastes can play an important role from the point of view of environment protection, and allowing to produce the valuable materials and energy [3-6].
Thermal degradation of natural and synthetic
Effect of temperature, heating rate and zeolite-based catalysts on the pyrolysis of high impact polystyrene (HIPS) waste ...
Polyolefins Journal, Vol. 6, No. 1 (2019)
polymers at high temperatures in the absence of oxygen (pyrolysis) can be a reliable solution to dispose polymeric wastes [7-8]. In pyrolysis process under high temperatures, high molecular weight chains are broken down into low molecular weight ones. Depending on the polymer type, with acceleration of the secondary reactions and the formation of hot spots, some cokes are also produced. Coke, amount of liquid and gas and composition of products from pyrolysis process depend on the different structural and process parameters, such as polymer type, temperature, catalyst, reactor, carrier gas and maybe some other unknown parameters [8-11].
Degradation mechanisms, including chain-stripping, cross-linking, un-zipping and chain scission are the known mechanisms for the thermal degradation of polymers. It appears that all of the above mentioned mechanisms happen in the pyrolysis process with different shares. The share of each mechanism depends strongly on the polymer type, though the process parameters, such as temperature, heating rate and catalyst type and ratio can affect the degradation mechanism perfectly [12-15].
Catalytic degradation of polymeric materials can control the degradation mechanisms and the catalyst used can be a key parameter in determining the type and size of the final pyrolysis products. The catalytic products of the hydrocarbonic polymers like HIPS are highly useful and can be utilized as fuels or chemicals in the various applications. In pyrolysis, zeolite catalysts lower the required energy and time obviously. A narrow variety of products depending on the pore size of catalyst is another advantage of catalytic pyrolysis in comparison with the thermal cracking [16-18].
Temperature as a critical and key parameter of pyrolysis plays an important role in determining the pyrolysis products, and high pyrolysis temperatures can decrease the role of catalyst. In sum, a review of the literature showed strong dependence of carbonization products to process parameters, such as temperature, catalyst type and polymer/catalyst ratio, heating rate and residence time [19-20].
Thermo-gravimetric analysis (TGA) is one of the commonly used techniques for consideration of degradation trend in terms of different process parameters, such as temperature, heating rate and etc. The effect of real parameters on the degradation mechanisms and activation energy can be studied by using TGA measurements. TGA can especially be used for study of the degradation behavior of polymer
materials, including homo-polymers, copolymers and etc., [13-15].
The goal of this paper is to elucidate the effect of temperature, heating rate and different zeolite-based catalysts on the pyrolysis of high impact polystyrene to produce the valuable products. Hence, we have reported the effect of zeolitic catalysts, such as used FCC (fluid catalytic cracking), HZSM-5 (hydrogen form Zeolite Socony Mobil–5) and Ga/used FCC, temperature and heating rate on the pyrolysis yield and the composition of the condensed products as well as the effect of heating rate on the degradation trend of HIPS using TGA method. Our results show that the studied parameters have a significant effect on the residence time, amount of produced styrene, the distribution of molecular weight, and the composition of condensed product. Also, the trend of degradation of HIPS does not change significantly in the range of studied heating rates.
Materials HIPS (7240 grade) was supplied by Tabriz Petrochemical Company, nitrogen gas (purity 99.99%) by Roham Co and spent FCC catalyst by Abadan FCC Refinery. Ga(NO3)2 was purchased from Merck Chemical, and HZSM-5 catalyst was supplied by Sudchemi Company.
Instruments and methods Catalyst preparation The spent FCC catalyst was regenerated at 650°C and steamed slightly for 4 hours. 0.78g Ga(NO3)2 was dissolved in distilled water (100g) under slow stirring at 90°C. The Ga/used FCC catalyst was prepared by the wetness incipient method. The Ga solution was added to the regenerated used FCC (30g) in a laboratory rotary dryer (RV8 model). The rotary temperature and rotation speed were raised step-by-step to obtain a dry mixture. Then, the Ga/used FCC was dried in an oven at 120°C for 16 hours, and then calcined for another 4 hours at 650°C prior to the experiment.
EDX A Quantax 200 energy-dispersive X-ray spectrometer (EDX) at a WD of 23.00 and 15 kV was used to detect the metals on the surface of used FCC, Ga/used FCC
Tamri Z., et al.
Polyolefins Journal, Vol. 6, No. 1 (2019)
and HZSM-5 catalysts. Furthermore, Si/Al ratio was calculated after detection of Al and Si elements.
BET BET (Brunauer–Emmett–Teller) method (Quantachrome Corp. Nova2200, Version 7.11) was used to calculate the surface area of the catalysts from the adsorption isotherms of nitrogen at 77K.
TGA Thermogravimetric analysis was performed on a Netzsch TG 209 thermo-balance. The initial mass of all the samples was 12.0-13.0 mg at the same sizes. The experiments were carried out in a nitrogen atmosphere (99.99% minimum purity) with a flow rate of 30 ml min-1.
Generally for polymer degradation, it is assumed that the rates of conversion are proportional to the concentration of reacted material. The rate of conversion can be expressed by the following basic rate equation:
)x(f)T(K T x
= ∂ ∂
b= ∂ ∂ (1)
Where "β" is the heating rate and "x" is the degree of advance defined by:
Where W is the weight of the sample at a given time t, W0 and Wf, refer to values at the beginning and the end of the weight loss event of interest, respectively. f(x) and K(T) are functions of conversion and temperature, respectively.
For each heating rate, the kinetic parameters, activation energy (Ea) and pre-exponential factor (A) of HIPS pyrolysis were determined by the integral method . Many investigators assumed that solid fuel pyrolysis is a first-order reaction [22–24].
GC/MS Identification of varied compounds in the condensed products was carried out by a gas chromatograph mass spectrometer (GC/MS) of model GC–MS-QP5000. The analysis was performed on a 60 m × 0.32 mm capillary column coated with a 1 µm f